analyical solutions for the automotive indus try 2017-07-07آ cds analytical analyical solutions...
Post on 11-Mar-2020
Embed Size (px)
CDS Analytical Analyical Solutions for the Automotive Industry
Modern polymers, including plastics and rubbers, hold the key to a host of safety and performance boosts in today’s automotive industry. Plastics currently make up 50% of the volume of new cars but only 10% of the weight, which helps make cars lighter and more fuel ef- ficient1. Novel plastic and rubber products also have improved passenger safety and auto designers rely on their versatility when designing new automobiles.
In addition to polymers, there has been improve- ment in paint technology. Although the newer paint styles may not have played a significant role in auto ef- ficiency, recent paint innovations have kept cars look- ing newer longer as well as becoming more environmentally friendly when applied.
Complex solid materials, like black rubber, automo- bile paint, fibers and plastics, may be examined using a variety of techniques. Several of them include solvent extraction, headspace-GC/MS and FTIR but, they can present a real challenge to obtain a full analysis of the total chemical makeup. The use of GC/MS can provide a wealth of information about complex chemical sys- tems, however the components usually must be volatile to be compatible with the technique.
Two “green analytical” techniques that can expand the use of any GCMS platform include pyrolysis and thermal desorption. Pyrolysis works by creating volatile compounds from seemingly incompatible ma- terials like tires, vinyl plastics and carpet fibers. Pre- cise heating of these samples at the GC inlet produces chromatograms, representing the various constituents of the sample, including additives, organic contami- nants and the polymers. Each polymer breaks down at high temperatures (typically above 400C) and will pro- vide a unique marker peak or pattern that can be used for identification.
Thermal Desorption can be utilized to concentrate volatile and semi-volatiles from air or a solid sample matrix. One major benefit is that they can increase the sensitivity of a standard GCMS by several orders of magnitude without the use of solvents or sample prep.
Also, heat can be applied (up to 350°C) on a solid sample which can be used to evolve and then trap semi-volatiles from large-solid samples.
The following examples represent several applica- tions within the automotive industry and their suppli- ers, using both of these techniques. They can be commonly applied in the R&D lab, for QC as well as in meeting developed methods, such as VDA-278. In addi- tion to the actual polymer identification, additives can be analyzed at low quantities including plasticizers, light stabilizers and antioxidants, among others.
Because it is so complex, comprised of many lay- ers, and usually contains opaque fillers such as metal flake and titanium dioxide, automobile paint is a very challenging analytical sample. Each layer is formulated for specific properties, and may include acrylics, epox- ies, urethanes and other polymer systems. Pyrolysis delivers the organic content to the GC/MS and leaves the inorganics behind, simplifying sample preparation.
Some analysts will prepare a sample of the entire paint, producing a complex pyrogram of the whole system, while others prefer to re-move the paint layer by layer and look at each one individually. Figure 1 shows the pyrogram made from a whole paint, and- contains peaks for several acrylics, plus a diisocyanate generated from a polyurethane. Figure 2 shows just a clearcoat, which also contains a variety of acrylic monomers, plus styrene. The 2-ethyl hexanol is probably a degradation product from the 2-ethylhexyl acrylate, and is sometimes seen in systems using DOP as a plasticizer.
continued on page 2.
Analytical Solutions for Polymers & Coatings in the Automotive Industry
1. American Chemistry Council
2. Methyl methacrylate
3. Butyl acrylate
4. Butyl methacrylate
5. Hydroxypropyl methacrylate
6. Octyl methacrylate
7. 5-isocyanato-1-(isocyanatomethyl) -1, 3, 3-trymethyl cyclohexane
Figure 1: Automobile Paint, Whole
CDS Analytical 2
The polymers used for rubbers, both natural and synthetic, are easily differentiated and analyzed using Py-GC/MS. In general, these polymers degrade to pro- duce some monomer, so the type of rubber is readily determined. In the case of natural rubber (polyiso- prene) the two largest peaks are for the monomer and the dimer of isoprene. Figure 3 shows the analysis of a synthetic automobile tire rubber formulated from bu- tadiene, isoprene and styrene, with an antioxidant (6PPD) added. Peaks are produced for each of the monomers used, and may provide quantitative infor- mation about the relative amounts of each.
Figure 4 shows a polyurethane rubber, different from the polyolefins. Nevertheless, it is easily identified as a polyurethane by the presence of the diisocyanate used. The polyol involved is a polyester type, using adipic acid, which produced the cyclopentanone peak. In this case, two different phthaltes are used as plasticizers.
Fiber blends are like other polymer blends or mix- tures when analyzed by Py-GC/MS in that the individ- ual polymers pyrolyze independently, and the resulting pyrogram contains pyrolysates from each of the con-
stituents. Figure 5 illustrates this process for a blend of Polyethylene terephthalate (PET) and Polyacrylonitrile (PAN). The top pyrogram in Figure 5 is PET only, showing the typical pyrolysis products, including benzoic acid, listed in Table 1. The bottom pyrogram is for PAN only, and has large peaks for acry- lonitrile monomer and dimer. The blended fiber is in the middle, and has the characteristic peaks of both the indi- vidual fibers. Since the pyrolysis prod- ucts of each polymer rarely interact with each other, comparing the amount of a product generated from one fiber to a compound from the other can be used
continued on page 5.
Figure 3: Synthetic Tire Rubber
1. Butalene monomer
2. Isoprene monomer
3. Bytadene dimer
5. Isoprene dimer
6. Antioxidant (6-PPD) (N-(1, 3-dimethylbutyl)- N’-phenyl-1, 4Benzendiamine)
Figure 4: Polyurethane Rubber
2. 1, 4-Butanediol
3. Methylene diphenyl disocyanate (MDI)
4. Benzyl butyl phthalate
5. Dioctyl phthalate
Figure 5: PAN/PET Fiber Blends
1. Vinyl benzoate
2. Benzoic acid
3. Divinyl terephthalate
4. Terephthalic acid monovinyl ester
6. Hexene dinitrile
3. Butyl methacrylate
4. 2 Ethyl hexanol
5. Hydroxypropyl methacrylate
6. 2 Ethylhexyl acrylate
7. Octyl methacrylate
Figure 2: Automobile Paint, Topcoat
CDS Analytical 3
Published Papers and Application Notes Published Papers
Automotive Paint Analysis using Pyrolysis-GC-TOFMS and Pyrolysis-GCxGC-TOFMS
LECO Corporation, St. Joseph, MI.
NHTSA Tire Aging Study using Pyrolysis GC-MS
Uday Karmarkar, Ana Barbur, Edward R. Terrill, Mark Centea, Larry R. Evans, James D. MacIsaac, Jr.
Akron Rubber Development Laboratory, Inc., Akron, OH
U.S. Dept. of Transportation Research Center, National Highway Traffic Safety Administration, Washington, DC
A Simple Polymer Identification Scheme
Paint & Coatings Industry Magazine
Thomas Wampler, Charles Zawodny, Karen Jansson, CDS Analytical, Oxford, PA
Recent Changes in Automotive Paint Formulation using Pyrolysis-Gas Chromatography/Mass Spectrometry for Identification
Journal of Analytical and Applied Pyrolysis
Gregory A. Bishea, FBI, Washington, DC
William J. Simonsick, E. I. DuPont de Nemours and Co., Philadelphia, PA
Thomas P. Wampler, CDS Analytical, Inc.
Analysis of Rubber Materials by Pyrolysis GC
Maxine Phair, Thomas Wampler, CDS Analytical, Inc.
Polymer Additive Analysis using Multi-Step Thermal Sampling-GC/MS
Thomas Wampler, CDS Analytical, Inc.
Multi-Step Thermal Characterization of Polymers Using GC/MS
T. P. Wampler, C. P. Zawodny, K. D. Jansson, CDS Analytical, Inc.
CDS Application Notes:
Pyrolysis-GC/MS of Polyurethanes
CDS Analytical App Note #71
Pyrolysis of Rubber with Antioxidant 6-PPD
CDS Analytical App Note #80
Analysis of a Layered Paint Sample using Pyrotomy
CDS Analytical App Note # 90
VDA 278 Analysis using Thermal Desorption with a GC/MS System
CDS Analytical App Note #97
Using a Thermal Technique to Extract Residual Oligomers
CDS Analytical App Note #110
Identifying Additives in a Pyrogram using Deconvolution Software
CDS Analytical App Note #113
Pyrolysis of the Bisphenol A Polymers Epoxy and Polycarbonate
CDS Analytical App Note #160
Pyrolysis-GC/MS in the Analysis of Fiber Blends
CDS Analytical App Note #162
Pyrolysis of Fluoropolymers Polyvinyl Fluoride vs. Polyvinylidine Fluoride
CDS Analytical App Note #164
CDS Analytical 4
CDS Users ACH-Glass Systems, MI
AGC Automotive Americas, MI
Akron Rubber Development Laboratory Inc., OH
AKZO Nobel Coatings Inc. MI
AKZO Nobel Ltda. Sao Paulo
Bodycote Testing Group - EXOVA, MI
Bridgestone Americas CRT, OH